# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_bo2823
_database_code_depnum_ccdc_archive 'CCDC 1519254'
_audit_update_record             
;
2016-11-25 deposited with the CCDC.
2017-01-27 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Ce2 I6 O18'
_chemical_formula_weight         1329.64

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   P2(1)

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   8.7252(17)
_cell_length_b                   7.0474(14)
_cell_length_c                   13.096(3)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.807(2)
_cell_angle_gamma                90.00
_cell_volume                     805.2(3)
_cell_formula_units_Z            2
_cell_measurement_temperature    153(2)
_cell_measurement_reflns_used    3531
_cell_measurement_theta_min      2.787
_cell_measurement_theta_max      31.489

_exptl_crystal_description       Prism
_exptl_crystal_colour            Yellow
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.04
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    5.484
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1156
_exptl_absorpt_coefficient_mu    17.180
_exptl_absorpt_correction_type   Multi-scans
_exptl_absorpt_correction_T_min  0.1266
_exptl_absorpt_correction_T_max  0.5847
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      153(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'Rotating Anode'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  AFC10/Saturn724+
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean 28.5714
_diffrn_standards_number         0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_decay_%        0
_diffrn_reflns_number            9720
_diffrn_reflns_av_R_equivalents  0.0418
_diffrn_reflns_av_sigmaI/netI    0.0737
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_theta_min         2.79
_diffrn_reflns_theta_max         31.49
_reflns_number_total             5245
_reflns_number_gt                4810
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0163P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   none
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00177(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.03(3)
_refine_ls_number_reflns         5245
_refine_ls_number_parameters     236
_refine_ls_number_restraints     13
_refine_ls_R_factor_all          0.0372
_refine_ls_R_factor_gt           0.0327
_refine_ls_wR_factor_ref         0.0652
_refine_ls_wR_factor_gt          0.0637
_refine_ls_goodness_of_fit_ref   0.979
_refine_ls_restrained_S_all      0.978
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ce1 Ce 0.35361(6) 0.52441(7) 0.29549(4) 0.00528(10) Uani 1 1 d . . .
Ce2 Ce 0.81951(6) 0.35920(7) 0.30206(4) 0.00535(10) Uani 1 1 d . . .
I1 I 0.11680(6) 0.41944(8) 0.50955(4) 0.00527(11) Uani 1 1 d . . .
I2 I 0.54663(7) 0.34682(10) 0.04771(4) 0.01024(12) Uani 1 1 d . . .
I3 I 0.69869(6) 0.86224(8) 0.20541(4) 0.00676(11) Uani 1 1 d . . .
I4 I 0.08257(6) 0.55581(9) 0.07091(4) 0.00575(11) Uani 1 1 d . . .
I5 I 0.17545(6) 0.03856(8) 0.19736(4) 0.00583(11) Uani 1 1 d . . .
I6 I 0.38585(6) 1.00372(8) 0.47208(4) 0.00519(11) Uani 1 1 d . . .
O1 O 0.3196(6) 0.3972(9) 0.4821(4) 0.0050(12) Uani 1 1 d . . .
O2 O 0.1824(7) 1.0307(9) 0.4949(4) 0.0075(12) Uani 1 1 d . . .
O3 O 0.4214(7) 0.9190(9) 0.6046(4) 0.0051(12) Uani 1 1 d . . .
O4 O 0.1194(7) 0.6632(9) 0.5491(5) 0.0080(13) Uani 1 1 d . . .
O5 O 0.2237(7) 0.4098(9) 0.1396(5) 0.0084(12) Uani 1 1 d U . .
O6 O 0.3946(7) 0.7740(9) 0.4113(5) 0.0070(13) Uani 1 1 d . . .
O7 O 0.5693(6) 0.3979(8) 0.1831(4) 0.0067(12) Uani 1 1 d . . .
O8 O 0.0727(7) 0.4616(9) 0.3731(4) 0.0090(13) Uani 1 1 d . . .
O9 O 0.0404(7) 0.4016(9) -0.0368(5) 0.0131(14) Uani 1 1 d . . .
O10 O 0.7604(8) 0.7054(9) 0.3065(5) 0.0108(14) Uani 1 1 d U . .
O11 O -0.0780(7) 0.5026(10) 0.1504(5) 0.0138(14) Uani 1 1 d . . .
O12 O 0.1800(7) -0.2123(9) 0.2298(5) 0.0115(14) Uani 1 1 d . . .
O13 O 0.5033(7) 0.7854(9) 0.1854(5) 0.0104(13) Uani 1 1 d . . .
O14 O 0.6669(7) 1.0670(9) 0.2830(5) 0.0117(13) Uani 1 1 d . . .
O15 O -0.0132(7) 0.0941(9) 0.2448(5) 0.0117(14) Uani 1 1 d . . .
O16 O 0.6715(8) 0.1416(10) 0.0429(5) 0.0148(15) Uani 1 1 d . . .
O17 O 0.2983(7) 0.1463(9) 0.2946(5) 0.0096(14) Uani 1 1 d . . .
O18 O 0.6626(8) 0.5299(10) -0.0044(5) 0.0165(14) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ce1 O6 2.347(6) . ?
Ce1 O5 2.457(6) . ?
Ce1 O3 2.459(5) 2_646 ?
Ce1 O12 2.538(6) 1_565 ?
Ce1 O7 2.565(6) . ?
Ce1 O1 2.624(6) . ?
Ce1 O13 2.687(6) . ?
Ce1 O8 2.704(7) . ?
Ce1 O17 2.708(6) . ?
Ce1 I1 3.5831(9) . ?
Ce2 O11 2.412(6) 1_655 ?
Ce2 O4 2.442(6) 2_646 ?
Ce2 O14 2.463(6) 1_545 ?
Ce2 O3 2.483(6) 2_646 ?
Ce2 O8 2.492(6) 1_655 ?
Ce2 O15 2.493(6) 1_655 ?
Ce2 O10 2.495(6) . ?
Ce2 O7 2.678(5) . ?
Ce2 O2 2.921(6) 2_646 ?
Ce2 I6 3.6257(9) 2_646 ?
I1 O4 1.794(6) . ?
I1 O1 1.817(6) . ?
I1 O8 1.846(6) . ?
I2 O18 1.781(7) . ?
I2 O16 1.813(6) . ?
I2 O7 1.818(6) . ?
I3 O14 1.789(7) . ?
I3 O10 1.801(6) . ?
I3 O13 1.805(6) . ?
I4 O11 1.797(6) . ?
I4 O9 1.815(6) . ?
I4 O5 1.831(5) . ?
I5 O15 1.810(6) . ?
I5 O12 1.819(6) . ?
I5 O17 1.819(6) . ?
I6 O6 1.806(6) . ?
I6 O2 1.814(6) . ?
I6 O3 1.857(6) . ?
I6 Ce2 3.6257(9) 2_656 ?
O2 Ce2 2.921(6) 2_656 ?
O3 Ce1 2.459(5) 2_656 ?
O3 Ce2 2.483(6) 2_656 ?
O4 Ce2 2.442(6) 2_656 ?
O8 Ce2 2.492(6) 1_455 ?
O11 Ce2 2.412(6) 1_455 ?
O12 Ce1 2.538(6) 1_545 ?
O14 Ce2 2.463(6) 1_565 ?
O15 Ce2 2.493(6) 1_455 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 Ce1 O5 147.95(19) . . ?
O6 Ce1 O3 76.6(2) . 2_646 ?
O5 Ce1 O3 134.3(2) . 2_646 ?
O6 Ce1 O12 75.9(2) . 1_565 ?
O5 Ce1 O12 72.09(19) . 1_565 ?
O3 Ce1 O12 150.4(2) 2_646 1_565 ?
O6 Ce1 O7 121.7(2) . . ?
O5 Ce1 O7 75.10(19) . . ?
O3 Ce1 O7 67.27(18) 2_646 . ?
O12 Ce1 O7 119.9(2) 1_565 . ?
O6 Ce1 O1 70.9(2) . . ?
O5 Ce1 O1 127.2(2) . . ?
O3 Ce1 O1 60.05(18) 2_646 . ?
O12 Ce1 O1 119.4(2) 1_565 . ?
O7 Ce1 O1 120.60(18) . . ?
O6 Ce1 O13 76.3(2) . . ?
O5 Ce1 O13 90.1(2) . . ?
O3 Ce1 O13 95.87(19) 2_646 . ?
O12 Ce1 O13 67.0(2) 1_565 . ?
O7 Ce1 O13 64.16(19) . . ?
O1 Ce1 O13 142.73(18) . . ?
O6 Ce1 O8 90.6(2) . . ?
O5 Ce1 O8 81.30(19) . . ?
O3 Ce1 O8 118.14(19) 2_646 . ?
O12 Ce1 O8 73.0(2) 1_565 . ?
O7 Ce1 O8 146.66(19) . . ?
O1 Ce1 O8 58.59(17) . . ?
O13 Ce1 O8 139.80(19) . . ?
O6 Ce1 O17 140.0(2) . . ?
O5 Ce1 O17 66.00(19) . . ?
O3 Ce1 O17 81.13(19) 2_646 . ?
O12 Ce1 O17 127.77(19) 1_565 . ?
O7 Ce1 O17 77.8(2) . . ?
O1 Ce1 O17 69.22(19) . . ?
O13 Ce1 O17 139.4(2) . . ?
O8 Ce1 O17 71.2(2) . . ?
O6 Ce1 I1 74.53(16) . . ?
O5 Ce1 I1 108.53(15) . . ?
O3 Ce1 I1 89.19(14) 2_646 . ?
O12 Ce1 I1 93.90(16) 1_565 . ?
O7 Ce1 I1 144.38(13) . . ?
O1 Ce1 I1 29.16(12) . . ?
O13 Ce1 I1 148.33(14) . . ?
O8 Ce1 I1 30.24(12) . . ?
O17 Ce1 I1 72.26(15) . . ?
O11 Ce2 O4 144.6(2) 1_655 2_646 ?
O11 Ce2 O14 118.2(2) 1_655 1_545 ?
O4 Ce2 O14 73.7(2) 2_646 1_545 ?
O11 Ce2 O3 131.4(2) 1_655 2_646 ?
O4 Ce2 O3 83.1(2) 2_646 2_646 ?
O14 Ce2 O3 74.4(2) 1_545 2_646 ?
O11 Ce2 O8 81.3(2) 1_655 1_655 ?
O4 Ce2 O8 71.5(2) 2_646 1_655 ?
O14 Ce2 O8 139.1(2) 1_545 1_655 ?
O3 Ce2 O8 121.3(2) 2_646 1_655 ?
O11 Ce2 O15 80.8(2) 1_655 1_655 ?
O4 Ce2 O15 72.2(2) 2_646 1_655 ?
O14 Ce2 O15 70.2(2) 1_545 1_655 ?
O3 Ce2 O15 141.2(2) 2_646 1_655 ?
O8 Ce2 O15 79.0(2) 1_655 1_655 ?
O11 Ce2 O10 71.8(2) 1_655 . ?
O4 Ce2 O10 125.3(2) 2_646 . ?
O14 Ce2 O10 135.1(2) 1_545 . ?
O3 Ce2 O10 69.3(2) 2_646 . ?
O8 Ce2 O10 83.7(2) 1_655 . ?
O15 Ce2 O10 149.5(2) 1_655 . ?
O11 Ce2 O7 77.7(2) 1_655 . ?
O4 Ce2 O7 133.5(2) 2_646 . ?
O14 Ce2 O7 65.86(19) 1_545 . ?
O3 Ce2 O7 65.17(17) 2_646 . ?
O8 Ce2 O7 154.0(2) 1_655 . ?
O15 Ce2 O7 112.17(19) 1_655 . ?
O10 Ce2 O7 75.3(2) . . ?
O11 Ce2 O2 125.7(2) 1_655 2_646 ?
O4 Ce2 O2 60.75(19) 2_646 2_646 ?
O14 Ce2 O2 115.3(2) 1_545 2_646 ?
O3 Ce2 O2 57.70(17) 2_646 2_646 ?
O8 Ce2 O2 63.68(19) 1_655 2_646 ?
O15 Ce2 O2 126.50(18) 1_655 2_646 ?
O10 Ce2 O2 64.56(19) . 2_646 ?
O7 Ce2 O2 118.18(17) . 2_646 ?
O11 Ce2 I6 138.36(17) 1_655 2_646 ?
O4 Ce2 I6 67.20(15) 2_646 2_646 ?
O14 Ce2 I6 92.57(16) 1_545 2_646 ?
O3 Ce2 I6 28.23(12) 2_646 2_646 ?
O8 Ce2 I6 93.42(15) 1_655 2_646 ?
O15 Ce2 I6 138.95(15) 1_655 2_646 ?
O10 Ce2 I6 66.53(16) . 2_646 ?
O7 Ce2 I6 92.16(13) . 2_646 ?
O2 Ce2 I6 29.76(11) 2_646 2_646 ?
O4 I1 O1 97.5(3) . . ?
O4 I1 O8 97.3(3) . . ?
O1 I1 O8 90.8(3) . . ?
O4 I1 Ce1 91.3(2) . . ?
O1 I1 Ce1 44.72(17) . . ?
O8 I1 Ce1 47.5(2) . . ?
O18 I2 O16 102.7(3) . . ?
O18 I2 O7 100.1(3) . . ?
O16 I2 O7 97.8(3) . . ?
O14 I3 O10 97.2(3) . . ?
O14 I3 O13 99.8(3) . . ?
O10 I3 O13 101.2(3) . . ?
O11 I4 O9 100.0(3) . . ?
O11 I4 O5 97.1(3) . . ?
O9 I4 O5 100.0(3) . . ?
O15 I5 O12 98.4(3) . . ?
O15 I5 O17 101.5(3) . . ?
O12 I5 O17 103.4(3) . . ?
O6 I6 O2 102.3(3) . . ?
O6 I6 O3 96.6(3) . . ?
O2 I6 O3 91.8(3) . . ?
O6 I6 Ce2 97.6(2) . 2_656 ?
O2 I6 Ce2 53.08(19) . 2_656 ?
O3 I6 Ce2 39.24(18) . 2_656 ?
I1 O1 Ce1 106.1(2) . . ?
I6 O2 Ce2 97.2(2) . 2_656 ?
I6 O3 Ce1 121.5(3) . 2_656 ?
I6 O3 Ce2 112.5(2) . 2_656 ?
Ce1 O3 Ce2 117.7(2) 2_656 2_656 ?
I1 O4 Ce2 140.7(3) . 2_656 ?
I4 O5 Ce1 121.5(3) . . ?
I6 O6 Ce1 161.7(3) . . ?
I2 O7 Ce1 123.9(3) . . ?
I2 O7 Ce2 128.6(3) . . ?
Ce1 O7 Ce2 107.5(2) . . ?
I1 O8 Ce2 119.1(3) . 1_455 ?
I1 O8 Ce1 102.3(3) . . ?
Ce2 O8 Ce1 135.3(2) 1_455 . ?
I3 O10 Ce2 130.0(3) . . ?
I4 O11 Ce2 150.0(3) . 1_455 ?
I5 O12 Ce1 143.2(3) . 1_545 ?
I3 O13 Ce1 126.3(3) . . ?
I3 O14 Ce2 130.1(3) . 1_565 ?
I5 O15 Ce2 143.5(3) . 1_455 ?
I5 O17 Ce1 121.1(3) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O6 Ce1 I1 O4 21.1(2) . . . . ?
O5 Ce1 I1 O4 -125.5(2) . . . . ?
O3 Ce1 I1 O4 97.4(2) 2_646 . . . ?
O12 Ce1 I1 O4 -53.1(2) 1_565 . . . ?
O7 Ce1 I1 O4 144.3(3) . . . . ?
O1 Ce1 I1 O4 99.4(3) . . . . ?
O13 Ce1 I1 O4 -2.5(3) . . . . ?
O8 Ce1 I1 O4 -98.7(3) . . . . ?
O17 Ce1 I1 O4 178.4(2) . . . . ?
O6 Ce1 I1 O1 -78.3(3) . . . . ?
O5 Ce1 I1 O1 135.1(3) . . . . ?
O3 Ce1 I1 O1 -2.0(3) 2_646 . . . ?
O12 Ce1 I1 O1 -152.5(3) 1_565 . . . ?
O7 Ce1 I1 O1 44.9(3) . . . . ?
O13 Ce1 I1 O1 -101.9(4) . . . . ?
O8 Ce1 I1 O1 161.9(4) . . . . ?
O17 Ce1 I1 O1 79.0(3) . . . . ?
O6 Ce1 I1 O8 119.7(3) . . . . ?
O5 Ce1 I1 O8 -26.9(3) . . . . ?
O3 Ce1 I1 O8 -163.9(3) 2_646 . . . ?
O12 Ce1 I1 O8 45.5(3) 1_565 . . . ?
O7 Ce1 I1 O8 -117.0(3) . . . . ?
O1 Ce1 I1 O8 -161.9(4) . . . . ?
O13 Ce1 I1 O8 96.2(4) . . . . ?
O17 Ce1 I1 O8 -83.0(3) . . . . ?
O4 I1 O1 Ce1 -84.2(3) . . . . ?
O8 I1 O1 Ce1 13.2(3) . . . . ?
O6 Ce1 O1 I1 92.4(3) . . . . ?
O5 Ce1 O1 I1 -57.2(4) . . . . ?
O3 Ce1 O1 I1 177.7(4) 2_646 . . . ?
O12 Ce1 O1 I1 31.9(3) 1_565 . . . ?
O7 Ce1 O1 I1 -151.4(2) . . . . ?
O13 Ce1 O1 I1 121.9(3) . . . . ?
O8 Ce1 O1 I1 -10.5(2) . . . . ?
O17 Ce1 O1 I1 -90.7(3) . . . . ?
O6 I6 O2 Ce2 90.3(3) . . . 2_656 ?
O3 I6 O2 Ce2 -6.9(3) . . . 2_656 ?
O6 I6 O3 Ce1 118.7(3) . . . 2_656 ?
O2 I6 O3 Ce1 -138.7(4) . . . 2_656 ?
Ce2 I6 O3 Ce1 -147.5(5) 2_656 . . 2_656 ?
O6 I6 O3 Ce2 -93.9(3) . . . 2_656 ?
O2 I6 O3 Ce2 8.8(3) . . . 2_656 ?
O1 I1 O4 Ce2 -81.1(5) . . . 2_656 ?
O8 I1 O4 Ce2 -172.8(5) . . . 2_656 ?
Ce1 I1 O4 Ce2 -125.5(5) . . . 2_656 ?
O11 I4 O5 Ce1 -81.7(4) . . . . ?
O9 I4 O5 Ce1 176.8(3) . . . . ?
O6 Ce1 O5 I4 -4.4(6) . . . . ?
O3 Ce1 O5 I4 -166.2(3) 2_646 . . . ?
O12 Ce1 O5 I4 -2.2(3) 1_565 . . . ?
O7 Ce1 O5 I4 -131.1(4) . . . . ?
O1 Ce1 O5 I4 111.5(4) . . . . ?
O13 Ce1 O5 I4 -67.9(4) . . . . ?
O8 Ce1 O5 I4 72.6(4) . . . . ?
O17 Ce1 O5 I4 145.9(4) . . . . ?
I1 Ce1 O5 I4 86.0(3) . . . . ?
O2 I6 O6 Ce1 58.8(12) . . . . ?
O3 I6 O6 Ce1 152.1(12) . . . . ?
Ce2 I6 O6 Ce1 112.5(11) 2_656 . . . ?
O5 Ce1 O6 I6 -2.2(15) . . . . ?
O3 Ce1 O6 I6 164.6(12) 2_646 . . . ?
O12 Ce1 O6 I6 -4.3(11) 1_565 . . . ?
O7 Ce1 O6 I6 112.4(11) . . . . ?
O1 Ce1 O6 I6 -132.8(12) . . . . ?
O13 Ce1 O6 I6 65.0(12) . . . . ?
O8 Ce1 O6 I6 -76.6(12) . . . . ?
O17 Ce1 O6 I6 -137.3(11) . . . . ?
I1 Ce1 O6 I6 -102.5(12) . . . . ?
O18 I2 O7 Ce1 111.2(4) . . . . ?
O16 I2 O7 Ce1 -144.4(3) . . . . ?
O18 I2 O7 Ce2 -69.0(4) . . . . ?
O16 I2 O7 Ce2 35.4(4) . . . . ?
O6 Ce1 O7 I2 -135.0(3) . . . . ?
O5 Ce1 O7 I2 15.0(3) . . . . ?
O3 Ce1 O7 I2 168.5(4) 2_646 . . . ?
O12 Ce1 O7 I2 -43.6(4) 1_565 . . . ?
O1 Ce1 O7 I2 139.7(3) . . . . ?
O13 Ce1 O7 I2 -82.5(3) . . . . ?
O8 Ce1 O7 I2 61.4(5) . . . . ?
O17 Ce1 O7 I2 83.1(3) . . . . ?
I1 Ce1 O7 I2 116.1(3) . . . . ?
O6 Ce1 O7 Ce2 45.1(3) . . . . ?
O5 Ce1 O7 Ce2 -164.9(3) . . . . ?
O3 Ce1 O7 Ce2 -11.4(2) 2_646 . . . ?
O12 Ce1 O7 Ce2 136.5(2) 1_565 . . . ?
O1 Ce1 O7 Ce2 -40.1(3) . . . . ?
O13 Ce1 O7 Ce2 97.7(2) . . . . ?
O8 Ce1 O7 Ce2 -118.4(3) . . . . ?
O17 Ce1 O7 Ce2 -96.8(2) . . . . ?
I1 Ce1 O7 Ce2 -63.7(3) . . . . ?
O11 Ce2 O7 I2 43.8(4) 1_655 . . . ?
O4 Ce2 O7 I2 -116.9(4) 2_646 . . . ?
O14 Ce2 O7 I2 -85.1(4) 1_545 . . . ?
O3 Ce2 O7 I2 -168.4(4) 2_646 . . . ?
O8 Ce2 O7 I2 80.7(6) 1_655 . . . ?
O15 Ce2 O7 I2 -30.8(4) 1_655 . . . ?
O10 Ce2 O7 I2 118.0(4) . . . . ?
O2 Ce2 O7 I2 167.9(3) 2_646 . . . ?
I6 Ce2 O7 I2 -177.0(3) 2_646 . . . ?
O11 Ce2 O7 Ce1 -136.4(2) 1_655 . . . ?
O4 Ce2 O7 Ce1 62.9(3) 2_646 . . . ?
O14 Ce2 O7 Ce1 94.7(3) 1_545 . . . ?
O3 Ce2 O7 Ce1 11.4(2) 2_646 . . . ?
O8 Ce2 O7 Ce1 -99.5(4) 1_655 . . . ?
O15 Ce2 O7 Ce1 149.0(2) 1_655 . . . ?
O10 Ce2 O7 Ce1 -62.2(2) . . . . ?
O2 Ce2 O7 Ce1 -12.3(3) 2_646 . . . ?
I6 Ce2 O7 Ce1 2.87(18) 2_646 . . . ?
O4 I1 O8 Ce2 -112.5(3) . . . 1_455 ?
O1 I1 O8 Ce2 149.8(3) . . . 1_455 ?
Ce1 I1 O8 Ce2 162.4(5) . . . 1_455 ?
O4 I1 O8 Ce1 85.1(3) . . . . ?
O1 I1 O8 Ce1 -12.6(3) . . . . ?
O6 Ce1 O8 I1 -56.8(3) . . . . ?
O5 Ce1 O8 I1 154.3(3) . . . . ?
O3 Ce1 O8 I1 18.3(4) 2_646 . . . ?
O12 Ce1 O8 I1 -131.9(3) 1_565 . . . ?
O7 Ce1 O8 I1 109.2(3) . . . . ?
O1 Ce1 O8 I1 10.2(2) . . . . ?
O13 Ce1 O8 I1 -126.0(3) . . . . ?
O17 Ce1 O8 I1 86.8(3) . . . . ?
O6 Ce1 O8 Ce2 145.2(4) . . . 1_455 ?
O5 Ce1 O8 Ce2 -3.7(4) . . . 1_455 ?
O3 Ce1 O8 Ce2 -139.7(3) 2_646 . . 1_455 ?
O12 Ce1 O8 Ce2 70.2(4) 1_565 . . 1_455 ?
O7 Ce1 O8 Ce2 -48.8(5) . . . 1_455 ?
O1 Ce1 O8 Ce2 -147.8(4) . . . 1_455 ?
O13 Ce1 O8 Ce2 76.0(5) . . . 1_455 ?
O17 Ce1 O8 Ce2 -71.2(4) . . . 1_455 ?
I1 Ce1 O8 Ce2 -158.0(6) . . . 1_455 ?
O14 I3 O10 Ce2 174.0(4) . . . . ?
O13 I3 O10 Ce2 72.4(5) . . . . ?
O11 Ce2 O10 I3 40.7(4) 1_655 . . . ?
O4 Ce2 O10 I3 -174.3(4) 2_646 . . . ?
O14 Ce2 O10 I3 -71.4(6) 1_545 . . . ?
O3 Ce2 O10 I3 -109.5(5) 2_646 . . . ?
O8 Ce2 O10 I3 123.6(5) 1_655 . . . ?
O15 Ce2 O10 I3 68.1(6) 1_655 . . . ?
O7 Ce2 O10 I3 -40.9(4) . . . . ?
O2 Ce2 O10 I3 -172.6(5) 2_646 . . . ?
I6 Ce2 O10 I3 -139.9(5) 2_646 . . . ?
O9 I4 O11 Ce2 109.6(7) . . . 1_455 ?
O5 I4 O11 Ce2 8.1(7) . . . 1_455 ?
O15 I5 O12 Ce1 -141.8(6) . . . 1_545 ?
O17 I5 O12 Ce1 -37.8(6) . . . 1_545 ?
O14 I3 O13 Ce1 -94.8(4) . . . . ?
O10 I3 O13 Ce1 4.7(4) . . . . ?
O6 Ce1 O13 I3 66.4(4) . . . . ?
O5 Ce1 O13 I3 -142.9(4) . . . . ?
O3 Ce1 O13 I3 -8.3(4) 2_646 . . . ?
O12 Ce1 O13 I3 146.6(5) 1_565 . . . ?
O7 Ce1 O13 I3 -69.5(4) . . . . ?
O1 Ce1 O13 I3 37.8(6) . . . . ?
O8 Ce1 O13 I3 140.6(3) . . . . ?
O17 Ce1 O13 I3 -91.5(4) . . . . ?
I1 Ce1 O13 I3 89.7(4) . . . . ?
O10 I3 O14 Ce2 105.5(4) . . . 1_565 ?
O13 I3 O14 Ce2 -151.8(4) . . . 1_565 ?
O12 I5 O15 Ce2 159.7(5) . . . 1_455 ?
O17 I5 O15 Ce2 54.0(6) . . . 1_455 ?
O15 I5 O17 Ce1 -79.4(4) . . . . ?
O12 I5 O17 Ce1 178.9(3) . . . . ?
O6 Ce1 O17 I5 145.3(3) . . . . ?
O5 Ce1 O17 I5 -10.5(3) . . . . ?
O3 Ce1 O17 I5 -158.0(4) 2_646 . . . ?
O12 Ce1 O17 I5 29.0(5) 1_565 . . . ?
O7 Ce1 O17 I5 -89.5(4) . . . . ?
O1 Ce1 O17 I5 140.7(4) . . . . ?
O13 Ce1 O17 I5 -69.3(5) . . . . ?
O8 Ce1 O17 I5 78.1(4) . . . . ?
I1 Ce1 O17 I5 110.0(4) . . . . ?

_diffrn_measured_fraction_theta_max 0.997
_diffrn_reflns_theta_full        31.49
_diffrn_measured_fraction_theta_full 0.997
_refine_diff_density_max         1.578
_refine_diff_density_min         -2.263
_refine_diff_density_rms         0.361
